Multifunctional Biocompatible Fluorescent 256 Multifunctional Biocompatible Fluorescent...
Embed Size (px)
Transcript of Multifunctional Biocompatible Fluorescent 256 Multifunctional Biocompatible Fluorescent...
Journal of Biomaterials and Nanobiotechnology, 2012, 3, 254-261 http://dx.doi.org/10.4236/jbnb.2012.322031 Published Online May 2012 (http://www.SciRP.org/journal/jbnb)
Multifunctional Biocompatible Fluorescent Carboxymethyl cellulose Nanoparticles
Ravindran Girija Aswathy, Balasubramanian Sivakumar, Dhandayudhapani Brahatheeswaran, Sreejith Raveendran, Tomofumi Ukai, Takahiro Fukuda, Yasuhiko Yoshida, Toru Maekawa, Dasappan Nair Sakthikumar*
Bio Nano Electronics Research Center, Graduate School of Interdisciplinary New Science, Toyo University, Kawagoe, Japan. Email: *firstname.lastname@example.org Received January 12th, 2012; revised February 24th, 2012; accepted March 10th, 2012
ABSTRACT A multifunctional nanoparticle based on Carboxymethyl cellulose was developed. Folate group was attached to nanoparti- cle for specific recognition of cancerous cells and 5FU was encapsulated for delivering cytotoxicity. The whole system was able to track by the semiconductor quantum dots that were attached to the nanoparticle. The multifunctional nanoparticle was characterized by UV-VIS spectra, PL spectra, FTIR, TEM, SEM etc and was targeted to human breast cancer cell, MCF7. The biocompatibility of nanoparticle without drug and cytotoxicity rendered by nanoparticle with drug was studied with MCF7 and L929 cell lines. The epifluorescent images suggest that the folate-conjugated nanoparti- cles were more internalized by folate receptor positive cell line, MCF7 than the noncancerous L929 cells. Keywords: Multifunctional; Carboxymethyl cellulose; Folate; Nanoparticles; Biocompatible
1. Introduction Bionanotechnology is an emerging and interdisciplinary research area developed as a result of synergistic combi- nation of nanotechnology and biotechnology . The new developments in bionanotechnology have emerged in various dimensions resulting concept of multifunc- tional nanoparticles to reality. The design and synthesis of “all in one approach” that integrate multiple nanoma- terials with different properties in a single nanosystem have several advantages when compared to single com- ponent with a single function [2-4]. The nanoparticles with an imaging moiety, with a potential drug to provide the cytotoxicity and a group or ligand to recognize the target cell can be one of the best examples for multifunc- tional nanoparticles [5-7]. Since cancer is considered to be one of the prime life threatening diseases in recent times, the multifunctional nanoparticles can play a sig- nificant role in the detection, monitoring and delivery of drug thereby treatment of cancer with much efficacy.
Cellulose is one among the most abundant biopoly- mers present in nature and cellulose based derivatives have several advantages such as biodegradability, recy- clability, reproducibility, cost effectiveness and avail- ability in a wide variety of forms. However, the poor solubility of cellulose in water and in most organic sol-
vents and also the poor reactivity make it difficult to fab- ricate directly to other useful materials. The derivative modification of cellulose can overcome these limitations while keeping the advantageous properties of cellulose. Carboxymethyl cellulose is a cellulose derivative with carboxymethyl groups (-CH2-COONa) bonded to some of the hydroxyl groups on cellulose backbone. It is one of the water-soluble cellulose derivatives with methyl group that has immense application in the food, pharmaceutical area owing to its viscosity, nontoxicity and hypoaller- genic nature . While making nanoparticles with Car- boxymethyl cellulose it provides carboxylic acid func- tionality to the nanoparticles and often used as a stabi- lizer for the synthesis of several other nanoparticles. The nanoparticles of carboxymethyl cellulose have several applications in cosmetic and pharmaceutical sector. The Carboxymethyl cellulose nanoparticles was made specific to cancer cells in our study by conjugating the folate group since folate recaptors are often over expressed in several cancers . The nanoparticle was then loaded with a potent anticancer drug, 5FU to form a semi multi- functional nanoparticle. The nanoparticles were con- verted to fully multifunctional nanoparticle when an im- aging moiety was attached to the nanoparticle . Rather than using an organic dye for imaging; we em- ployed semiconductor quantum dots (QD) for providing luminescence for our nanoparticle. Semiconductor QDs *Corresponding author.
Copyright © 2012 SciRes. JBNB
Multifunctional Biocompatible Fluorescent Carboxymethyl cellulose Nanoparticles 255
have several advantages than organic dyes such as non- photo bleaching with narrow, symmetric emission spec- tra, and have multiple resolvable colors that can be ex- cited simultaneously using a single excitation wavelength [11-14].
The multifunctional nanoparticle was characterized, imaged and biocompatibility of nanoparticle was also de- termined. Human breast cancer cell line MCF7 and a normal mouse fibroblast cell line, L929 was used in our study. The multifunctional nanoparticle was targeted to human breast cancer cell line and the cytotoxicity ren- dered by the drug in the nanoparticle was studied by cell viability assays. The intake of nanoparticle was studied by epifluorescent images and by flow cytometry studies.
2. Materials and Methods 2.1. Chemicals Zinc acetate, manganese sulfate, calcium chloride, car- boxymethyl cellulose was purchased from Kanto Che- micals, Japan. Sodium sulfide 9 H2O and folic acid were procured from Sigma-Aldrich, (St. Louis, MO, USA). N- (3-Dimethyl aminopropyl)-N0-ethylcarbodiimidehydro- chloride (EDC), N-hydroxysuccinimide (NHS) were pro- cured from Tokyo Chemical Industries, Japan and 2,4- dihydroxy-5-fluorpyrimidin (5-FU) were purchased from Nacalai tesque, Inc., Japan.
2.2. Synthesis of Free and Drug-Loaded Folate Conjugated Fluorescent Carboxymethyl cellulose Nanoparticles
The multifunctional drug loaded folate conjugated fluo- rescent Carboxymethyl cellulose nanoparticles was pre- pared by 3 steps.
2.2.1. Synthesis of Folate Conjugated Carboxymethyl cellulose Nanoparticles
Folic acid (1 mg/ml) was prepared and the carboxyl groups on the surface was functionalized with N-(3-Di- methyl aminopropyl)-N0-ethylcarbodiimidehydrochlo- ride (EDC) (0.78 mg) and N-hydroxysuccinimide (NHS) (0.98 mg) and was allowed to stir for 2 h at room tem- perature. 5 mg/ml Carboxymethyl cellulose was prepared and 25 ml was added drop by drop to the above mixture and was allowed to stir overnight. Ionic cross-linking of folate conjugated Carboxymethyl cellulose mixture was achieved by adding CaCl2 (1%) to yield drug free nanoparticles.
2.2.2. Synthesis of Drug-Loaded Folate Conjugated Carboxymethyl cellulose Nanoparticles
5FU (2 mg) was dissolved in methanol and was added drop by drop to folate conjugated Carboxymethyl cellu- lose mixture and was kept stirring for 1 hour to evaporate
methanol. CaCl2 (1%) was added for cross-linking and mixture was allowed to stir for 30 minutes.
2.2.3. Synthesis of Fluorescent Nanoparticles ZnS:Mn QDs was prepared via previously reported meth- od . Briefly Zinc acetate (0.1 M) was dissolved in10 ml deionized water and N2 was purged for 10 minutes. Manganese sulphate, (0.01 M), 1 ml was added drop-by- drop and kept stirring for 10 minutes. 10 ml of 0.1 M Sodium sulphide was added slowly and continued stir- ring for another 30 minutes. The fluorescence from the sample was observed in an UV lamp at 365 nm excita- tion energy and the sample exhibited typical orangish red emission. The as synthesized QD was added drop-by- drop to folate-conjugated drug loaded and drug free car- boxymethyl cellulose. The process was continued until the nanoparticles exhibited sufficient fluorescence. The drug free resulting reaction mixture was centrifuged, washed twice with deionized water and lyophilized to get fine yellow powder that was used for characterization studies.
2.3. Characterization of Nanoparticles The UV-VIS spectra of nanoparticles were measured us- ing a Shimadzu UV-VIS spectrophotometer (UV-2100- PC/3100 PC). The absorbance of QD, folate conjugated Carboxymethyl cellulose and 5FU folate conjugated car- boxymethyl cellulose nanoparticles were recorded. PL spectra were recorded with a F-4500 fluorescent spec- trophotometer, Hitachi, Japan at an excitation wave- length of 360 nm. TEM images of QD were acquired by JEM-2200-FS Field emission transmission electron mi- croscope (JEOL, Japan) to an operating voltage of 200 kV. The grids were given hydrophilic treatment using Joel Datum HDT-400 hydrophilic treatment device. TEM samples were prepared by dropping the diluted QDs into the carbon coated hydrophilic copper TEM grids. The SEM images of 5FU encapsulated folate conjugated Carboxymethyl cellulose QD nanoparticles were taken by Scanning Electron Microscope (JEOL, JSPM-6490, Ja- pan). Nanoparticle suspension was diluted with ultra pure water and dropped on silica substrate, dried under vac- uum and the images were acquired. AFM image of nanoparticle was performed in MFP3D Asylum Research. FTIR spectroscopic analysis of Carboxymethyl cellulose, folic acid, 5FU, QD and lyophilized composite, 5-FU loaded folic acid conjugated Carboxymethyl cellulose was recorded on Perkin Elmer spectrophotometer in the spectral range of 4000 to 400 cm–1 at room temperature. The data sets were averaged over 32 times. The thermo- gravimetric analysis (TGA) of Carboxymethyl cellulose, QD and nanoparticle was carried out in DTG-60H, Shi- madzu thermal analyzer. TGA of all the s